- Home
- Documents
*Prediction of Lightweight Aggregate Concrete Compressive ... · PDF file compressive strength...*

Click here to load reader

View

6Download

0

Embed Size (px)

Journal of Rehabilitation in Civil Engineering 6-2 (2018) 154-163

DOI: 10.22075/JRCE.2017.11556.1192

Journal homepage: http://civiljournal.semnan.ac.ir/

Prediction of Lightweight Aggregate Concrete

Compressive Strength

O. Fatahi 1 and S. Jafari

2*

1. M.Sc., Discipline of Civil Engineering, Islamic Azad University, Eyvan-e-Gharb Branch, Eyvan, Iran

2. M.Sc., Department of Civil and Environmental Engineering, Shiraz University of Technology, Shiraz, Iran

Corresponding author: [email protected]

ARTICLE INFO

ABSTRACT

Article history:

Received: 07 June 2017

Accepted: 05 September 2017

Nowadays, the better performance of lightweight structures

during earthquake has resulted in using lightweight concrete

more than ever. However, determining the compressive

strength of concrete used in these structures during their service through a none-destructive test is a popular and

useful method. One of the most original approach of non-

destructive testing to obtain of compressive strength of

concrete used in structures is ultrasonic pulse velocity test.

The purpose of this research is predicting the compressive

strength of LWA concrete by proposing an accurate

mathematical formulation. Many samples of lightweight

aggregate concrete, made by expanded clay, have been

produced and tested. After determining the actual

compressive strength and indirect ultrasonic pulse velocity

for each sample, a relationship was derived to estimate the

compressive strength through Gene Expression

Programming (GEP). The results show the presented

equation shows high accuracy in predicting the compressive

strength of LWA and the estimated outcomes have a

considerable compatibility with actual samples.

Keywords:

Lightweight Aggregate

Concrete,

Gene Expression Programming,

Ultrasonic Pulse Velocity,

None-Destructive Test,

Prediction of Compressive

Strength.

1. Introduction

Lightweight concrete can be defined as a

type of concrete which includes an

expanding agent in that it increases the

volume of the mixture while giving

additional qualities such as reliability and

lessened the dead weight [1]. It is lighter than

the conventional concrete with a dry density

of 300 kg/m3 up to 1840 kg/m3; 87 to 23%

lighter. It was first introduced by the Romans

in the second century where ‘The Pantheon’

has been constructed using pumice, the most

common type of aggregate used in that

particular year [2]. The main specialties of

lightweight concrete are its low density and

thermal conductivity. Its advantages are that

there is a reduction of dead load, faster

building rates in construction and lower

haulage and handling costs [3]. A large

https://dx.doi.org/10.22075/jrce.2017.11556.1192 http://civiljournal.semnan.ac.ir/

O. Fatahi and S. Jafari/ Journal of Rehabilitation in Civil Engineering 6-2 (2018) 154-163 155

number of users acknowledge the profits of

this materials as they suggest flexibility in

design and impressive cost savings [4-7].

As the lightweight concrete can decline the

weight of earthquake resistant structures with

many applications, many researchers have

conducted a considerable number of

researches on the Specification and behavior

of various sort of LWA concretes [8, 9].

Using non-destructive methods for

evaluating the properties of concrete needs

high accuracy relationships, moreover many

of these relationships are not suitable for all

types of concrete require a different

calibration comparing other types of

concrete, which can be considered as the

main effect of these methods. On the other

hand, evaluation the concrete properties such

as compressive strength in the service area

through non-destructive tests has a growing

popularity, because these method are easy to

conduct and low cost and time saving.

Moreover, UT is One of the most original

approach of non-destructive testing to obtain

of compressive strength of concrete used in

structures. Therefore, much research has

been done on the combination of non-

destructive methods to improve evaluation.

But, the problems of preparing calibration

graphs for every kind of concrete have been

used still remains. In this regard,

considering mentioned problems, the use of

mathematical and evolutionary models such

as fuzzy logic, neural networks, artificial

intelligence and GA which can be managed

based on empirical studies have been

developed [10-14].

Gene Expression Programming (GEP) is

capable of solving user-defined problems

through computer programs which is a

progressive Evolutionary Algorithm (EA)

[14, 15]. In GEP, computer programs are

typically encoded by fixed-length gene

expression strings that are evolved through

nature-inspired operators such as mutation

and crossover. Nowadays, GEP is defined as

a powerful method in finding accurate and

concise equations [15, 16]. It has been used

in many actual applications with acceptable

success reported, including time series

predictions [17], classification problems [15],

regression problems [15], data mining and

knowledge discovery [18-20], etc.

It is necessary first to give feedback on the

ultrasonic tests on concrete that may be the

most important non-destructive test on the

concrete. By conducting multiple tests on

concrete samples made of different kinds of

aggregates, Facaoaru has provided the pulse

velocity ranges with considering the kind of

the aggregates [21]. Malhotra has

investigated the pulse velocity of samples of

concrete made with different water-cement

proportions and diverse aggregates [22].

Gaydecki investigated the propagation and

attenuation of ultrasonic pulses in samples

[23]. Manish et al., and Kewalramani and

Gupta in the separate studies, through

artificial neural networks and using UT,

predicted the compressive strength of

concrete and compared the outcomes

of neural networks and multiple variable

regressions [12, 24]. Trtnik et al. suggested a

model for predicting the compressive

strength of concrete based on UT and

Programming in MATLAB [10, 13]. Using

GEP, Mousavi et al. offered a new model for

estimating the compressive strength of high

performance concrete [25]. Fakharian et al.

presented a model for compressive strength

prediction of FRP-Confined rectangular

columns based on GEP [26]. Using GEP,

Ebtehaj and Bonakdary presented a model to

predict sediment transport in sewer [27].

156 O. Fatahi and S. Jafari/ Journal of Rehabilitation in Civil Engineering 6-2 (2018) 154-163

Hadianfard and Jafari proposed some

mathematical equations to estimate the

compressive strength of LWA concrete using

from the ultrasonic pulse velocity testing

outcomes obtained from gene expression

programming [10].

Regarding to increasing importance and

application of structural lightweight

aggregate concrete, this paper proposed a

equation to calculate the compressive

strength of the concrete by indirect ultrasonic

testing method which is a non-destructive

test where elevation of direct ultrasonic pulse

velocity is not possible. The important results

of this study are as follows: The model is

simple to use, easy to use and relatively low

cost to gain strength lightweight concrete

which is not studied yet.

2. Experimental Program

To reach the aim of this paper, more than 32

batch of LWAC have been produced and

tested. The location of laboratory was Shiraz

University of Technology. The properties of

Expanded Clay as the LWA used as well as

determination of the LWAC mixing ratio

were based on the ASTM C330 [28] and ACI

211.2 [29], respectively. Even though certain

differences, especially in proportioning and

batching procedures are observed which is

important to be notified to make a high

quality finished product, the other steps are

similar to the procedures for normal weight

concrete [30, 31].

2.1. Material Proportion and Mix Design

Fineness modulus of the modified fine sand

after sifting and amendment was 3.

Moreover, the experiments undertaken

the sand moisture content was 1%. In

addition, the specific gravity of the fine sand

was 1717.65Kg/m 3 , which was determined in

base on ASTM C 29 [32]. In the mix design,

the saturated surface dry (SSD) condition for

the sand measured 6% water.

The gradation of aggregates was in

accordance with the mentioned requirements

mentioned in ASTM C 330 [